Outline Asphalt Binders Asphalt Emulsions Cutback Asphalts Polymer Modified Binders and Performance Based Asphalt Asphalt Rubber Aggregates Storage and Handling Sampling Guidelines and Delivery
Asphalt Binders Paving Asphalt Constituent A complex hydrocarbon mixture consisting primarily of the residue from crude oil refning Asphalt properties depend on its chemical composition, crude source and type Highly temperature dependent Caltrans requirements for asphalt binders – Section 92 of the Standard Specifications
Asphalt Binders – Specifications Caltrans used AR (Aged Residue) system for many years Caltrans adopted the Performance Graded (PG) system for asphalt binder since 2006 for conventional binders and 2007 for modified binders
Asphalt Binders – Specifications In the PG system, asphalt is specified by: Dynamic Shear Rheometer (DSR) for performance at high and intermediate temperatures Bending Beam Rheometer (BBR) for performance at cold temperatures Aging Characteristics Purity and Safety
Asphalt Binders – Specifications EquipmentPurposePerformance Parameter Rolling Thin Film Oven, RTFO Simulate binder aging during HMA production & construction Resistance to aging during and immediately after construction Pressure Aging Vessel, PAV Simulate binder aging during HMA life Resistance to aging over the length of pavement service life Rotational Viscometer, RV Measure binder properties at high construction temperature Handling & pumping Dynamic Shear Rheometer, DSR Measure binder properties (stiffness and elasticity) at high and intermediate service temperatures Resistance to permanent deformation (rutting) and fatigue cracking Bending Beam Rheometer, BBR Measure binder properties at low service temperatures Resistance to thermal cracking
Performance Graded Asphalt Binder Specification Grade PropertyAASHTO Test Method PG a PG PG PG PG Original Binder Flash Point, Minimum °CT48230 Solubility, Minimum % b T4499 Viscosity at 135°C, c Maximum, Pa·s T Dynamic Shear, Test Temp. at 10 rad/s, °C Minimum G*/sin(delta), kPa T RTFO Test e, Mass Loss, Maximum, % T RTFO Test Aged Binder Complete table available at Asphalt Binders – Specifications - Unmodified
Binder Climatic Region Conventional AsphaltRubberized Asphalt Dense Graded Open Graded Gap Graded Open Graded TypicalSpecial PG PBAPGPBA 2 PG South Coast Central Coast Inland Valleys a(mod)64-106a64-16 North Coast64-16N/A6a(mod)64-166a64-16 Low Mountain South Mountain 64-16N/A6a(mod)64-166a64-16 High Mountain High Desert 64-28N/A6a, 6b64-286a58-22 Desert70-10N/A 6a(mod), a64-16 Asphalt Binders – Specifications - Unmodified
Complete table available at Asphalt Binders – Specifications - Modified
Asphalt Emulsions Emulsion Constituent An asphalt dispersed in water Breaking The process of separating the asphalt and water Curing The process by which the asphalt expels water and dries to a film on the aggregate or surface
Asphalt Emulsions Emulsion Manufacture Asphalt is sheared into small droplets and coated/reacted with a chemical stabilizer or emulsifier Emulsion must be stored at right pressure and temperature to prevent from damaging
Asphalt Emulsions A device used to shear the asphalt – Colloid Mill Cross
Asphalt Emulsions Emulsion plant operations
Asphalt Emulsions Emulsifiers Anionic emulsifiers are based on fatty acids Cationic emulsifiers are based on various types of amines. Cationic emulsifiers are used for slow set, rapid, quick sets and micro surfacing of various types of amines depending on the application. Caltrans uses both. The choice between anionic and cationic is based on the application requirements and the characteristics of the aggregate to be used in the mix
Asphalt Emulsions Caltrans Specifications Anionic emulsions: rapid set (RS), Medium Set (MS), and Slow Set (SS) Cationic emulsions: rapid set (CRS), Medium Set (CMS), and Slow Set (CSS) Subcategories Polymer modified emulsions Quickset slurry emulsion
Cutback Asphalts A solution of asphalt in a hydrocarbon solvent (e.g., kerosene, diesel, or naphtha) Solvents are used to reduce the asphalt’s viscosity so that the cutback can be pumped and sprayed at lower temperatures (104 to 293 F [40 to 145ºC]) than that required for conventional asphalt
Cutback Asphalts In California, only slow and medium cure cutbacks are still made and only slow cure cutbacks are generally specified The main use for cutbacks is prime coats over aggregate base materials prior to placement of an asphalt-wearing course in new construction
Cutback Asphalts Manufacture Easy Manufactured on site by circulation in a tank In refinery Specifications and Testing Standard specifications Section 93 “Liquid Asphalts” Flash point and water content, viscosity, and boiling range of the solvent
Polymer Modified Binder Polymers large molecules that are used to enhance the performances of asphalt cement and asphalt concrete pavement, particularly at high temperatures. Specifications and Testing Polymer Modified Binders Styrene Butadiene Copolymer (radial and linear) (SBS) Polyethylene (PE) Styrene Butadiene Rubber (SBR) Polybutadiene (PB) Ethylene Vinyl Acetate (EVA) Ehtylene Methyl Acrylate (EMA) Atactic Polypropylene (PP) Epoxies and Urethanes Tire Rubber (Crumb)
Polymer Modified Binder Manufacture Procedures Metering of polymer, asphalt, and additives. Wetting of the polymer by the asphalt/additive blend. Dispersion of the polymer. Allowance for any interaction (reaction) of the polymer with the asphalt. Storage and transportation Most important steps are dispersion and reaction
Complete table available at Polymer Modified Binder
Asphalt Rubber Asphalt Rubber Constituent Crumb Rubber Modifier (CRM) Scrap Tire Rubber High Natural Rubber Content Scrap Rubber Asphalt Cement Extender oil - Caltrans Asphalt rubber manufacture Heat asphalt cement to ~ 375 to 440°F Add CRM into a pre-wet tank Asphalt contacts and wets CRM particles Asphalt reacts with rubber particles to form a gel coated particle
Crumb Rubber Modifier (CRM) SCRAP TIRE 1/16” +/- in Size HIGH NATURAL RUBBER 1/32” +/- in Size
Without extender oilWith extender oil
AR PG Asphalt Cements For high mountain and high desert areas, use PG as the base asphalt. For other areas (coastal, inland valleys, low and south mountain, and low desert) use PG as base asphalt.
AR Binder Specification ARB: 20 2% CRM content by total binder mass. The CRM must include 25 2% by mass of high natural rubber CRM and 75 2% scrap tire CRM. The scrap tire CRM consists primarily of No. 10 to No. 30 sized particles (2 mm to 600 m sieve sizes). The high natural rubber CRM is somewhat finer, mostly No. 16 to No. 50 (1.18 mm to 300 m sieve sizes).
AR Binder Specification The extender oil dosage for chip seals ranges from 2.5 to 6% by mass of the asphalt cement. However, the minimum extender oil content for use in RAC mixes may be reduced to one percent to minimize potential for flushing and bleeding for hot climate, high traffic index (TI) locations.
Aggregates The major building material for pavements Form the structural matrix in AC mix Types Igneous Sedimentary rocks Gravel Sands Slag
Aggregate Properties Chemical Affinity to asphalt Physical Grading or particle size distribution Cleanliness or presence of deleterious materials Hardness or abrasion resistance Durability or soundness Particle shape and surface texture Absorption characteristics
Storage and Handling Conventional asphalt Modified asphalts, including asphalt rubber and MB) Asphalt emulsions Aggregate
Storage and Handling Conventional asphalt Avoiding Problems during Storage Minimizing the risk of overheating Minimizing oxidation and loss of volatiles Maintaining asphalt homogeneity Minimizing heat loss Storage and Handling Temperatures and Times are product specific
Storage and Handling Asphalt Emulsion Handling Pumping – use of appropriate pump to avoid changing the properties of emulsion Temperature – affects the behavior of asphalt droplets Transport – avoid air enters the emulsion since air can break the emulsion Do not mix cationic and anionic emulsions Storage The key is to prevent asphalt particles from settling
Storage Product Mixing Temperature ºF (ºC) Spraying Temperature ºF (ºC) Storage Temperature ºF (ºC) RS-1N/A (20-60) RS-2N/A (20-60) (50-85) MS (10-70) (20-70) (20-60) MS (10-70)N/A (50-85) MS-2h (10-70)N/A (50-85) SS (10-70) (10-60) SS-1h (10-70) (10-60)
Storage and Handling Tankage Guidelines Bulk tanks should be circulated at regular intervals. Circulation should be done slowly. The frequency of circulation will depend on the weather and how long the emulsion has spent in storage. Most emulsions only require circulation once a week in summer and once every five days during the winter. Circulation should be performed in the middle of the day, not first thing in the morning due to the colder temperatures.
Storage and Handling Tankage Guidelines The time of circulation is based on the size of the tank; a 1320 gal (5000 L) tank should be circulated for 15 minutes while a 2640 gal (10,000 L) tank requires 20 minutes. Pumps must be flushed after use, but never into the emulsion tank. Lines and pumps should be able to be warmed before use. Lines should not be left part full of emulsion.
Storage and Handling Cleaning Procedures Flush equipment including hoses thoroughly with WATER. Flush equipment and hoses with kerosene, NOT diesel, distillate or other solvent. These materials may dissolve asphalt but they are also incompatible with the emulsion and may cause the emulsion to break rather than flush it away. NEVER FLUSH INTO THE EMULSION TANK.
Storage and Handling Cleaning Procedures (cont.) Finish with a second flush with water. If a pump or line is already clogged with bitumen gentle heat may be applied at the blockage. Do not apply heat to the lines, as this will break the emulsion. Soak pumps with kerosene for an hour or more. Flush again with water after blockage is removed.
Acceptable Switch Load Combination Last Product in Tank Product to be Loaded Asphalt CementCutback Asphalt Cationic Emulsion Anionic Emulsion 꿀 Asphalt Cement OK to Load Empty to No Measurable Quantity Cutback Asphalt Empty to No Measurable Quantity OK to Load Empty to No Measurable Quantity Cationic Emulsion Empty to No Measurable Quantity OK to Load Empty to No Measurable Quantity Anionic Emulsion Empty to No Measurable Quantity OK to Load Crude Petroleum and Residual Fuel Oils Empty to No Measurable Quantity Any Product Not Listed Above Tank Must be Cleaned
Aggregate Storage and Handling Stockpile areas should be clean and stable to avoid contamination from the surrounding area. Stockpiles should be on free draining grades to avoid moisture entrapment. Stockpiles should be separated for different aggregate sizes to prevent inter-mingling.
Aggregate Storage and Handling Segregation may be avoided by avoiding stockpiling in a cone shape. Acceptable stockpile shapes are either horizontal or radial. Making each end dump load a separate pile, each adjacent to the next, makes horizontal stockpiles. Radial stockpiles are made with a radial stacker. Degradation of the aggregate creating fines can be avoided by handling the stockpile as little as possible. In chip seal or slurry surfacing applications, re-screening may be considered.
Sampling Guidelines Samples of emulsion and binder shall be taken in conformance with the requirements in AASHTO T 40, “Sampling Bituminous Materials,” and Section and 8-02 of the Construction Manual and California Test Method 125 Observe safety procedures Sample binders daily using new, clean, dry 0.26 gal (1 L) cans with screw lids Samples are normally taken from the application lance at the rear of the distributor. Drain off sufficient material through the nozzle to ensure removal of any material lodged there
Sampling Guidelines Samples should be taken after one-third and not more than two-thirds of the load has been removed Do not submerge sample containers in solvent or wipe containers with solvent saturated cloths. Use a clean, dry cloth, only immediately after sampling, to clean containers Attach a Sample Identification Form (TL-0101) to each material sample in accordance with Section of the Construction Manual and instructions printed on the TL-0101 booklet Provide the address of the Resident Engineer on the TL-0101
Sampling Guidelines Emulsions have a shelf life; therefore, it is important that all samples be sent to the Transportation Laboratory daily Aggregates should be sampled according to the contractual requirements Samples of aggregate shall be taken according to Section “Proportioning” of the Standard Specifications Samples may be taken from a conveyor belt or sampling chute. Field samples must be taken from the stockpile. AASHTO T 2 and Section of the Standard Specifications (9) describe the method
Sample Delivery Samples for testing are to be delivered to the Transportation Laboratory: Materials Engineering and Testing Services Flexible Pavement Materials Branch, MS # Folsom Boulevard Sacramento, California
Summary Asphalt Binders Asphalt Emulsions Cutback Asphalts Polymer Modified Binders and Performance Based Asphalt Asphalt Rubber Aggregates Storage and Handling Sampling Guidelines and Delivery